Ames Laboratory ISC Technical Reports Ames Laboratory
The ferromagnetic properties of the rare earth
J. F. ElliottIowa State College
Sam LegvoldIowa State College
F. H. SpeddingIowa State College
Follow this and additional works at:http://lib.dr.iastate.edu/ameslab_iscreports Part of theChemistry Commons
This Report is brought to you for free and open access by the Ames Laboratory at Iowa State University Digital Repository. It has been accepted for inclusion in Ames Laboratory ISC Technical Reports by an authorized administrator of Iowa State University Digital Repository. For more information, please email@example.com.
Elliott, J. F.; Legvold, Sam; and Spedding, F. H., "The ferromagnetic properties of the rare earth metals" (1953).Ames Laboratory ISC Technical Reports. 48.
The magnetic moment of gadolinium was measured in applied fields of 4,000-18,000 oersteds, and over the temperature range of 20.4°K to 320°K.
Keywords Ames Laboratory
UNITED STATES ATOMIC ENERGY COMMISSION
THE FERROMAGNETIC PROPERTIES OF THE
RARE EARTH METALS
J.F. Elliott Sam Legvold F. H. Spedding
Information Service, Oak Ridge, Tennessee
This report has been reproduced directly from the best evaileble copy.
R6production of this information is encouraged by the United States Atomic Energy Commission. Arrangements for
your republication of this document in whole or in part should be made with the author and the organization he
Issuance of this document does not constitute authority
TABIE OF CONTENTS
EXPERIMEN'l'•lL PROCEDURE •
Materials Method of Appa.rd.tus
• • Heasurement
.• • • • • •
rl o RESULTS
Gadolinium • Dysprosium •
Erbium • •
Vo DISCUSSION OF HESULTS
Gadolinium • Dyspro si urn •
Discussion of Errors General
.• • • •
• • 0
VI. LITERATURE CITED •
VII. APPENDICES •
A. Gadolinium •
1. Measured values of the magnetic moment of
2. Saturation magnetic moment of gadolinium
at T°K • • •
1. Measured values of the ~gnetic moment of
dysprosium • • •
2. saturation magnetic moment of dysprosium
d.t T°K •
C. Erbium •
l. J~asured values of the magnetic moment of erbium
THE FERROMAGNETIC PROPERTIES OF THE RARE EARTH METALS*
J. F. Elliott, Sam Legvold and F. H. Spedding
The magnetic moment of gadolinium was measured in applied fields of 4,000-18,000 oersteds, and over the temperature range of 20.4°K to 320°K.
The ferroma?netic absolute saturation moment of gadolinium was found to be 2)3.6-0.9 cgs units, confirming the work of Trombe (18, 19). This absolute saturation moment corresponds to abdut 7.12 Bohr magnetons.
The Curie point for gadolinium was determined by two different methods. The two determinations do not agree.
The magnetic moment of dysprosium was measured in applied fields of 43000-18,000 oersteds, and over the temperature range of 20.4°K to 20)°K.
The susceptibility of dysprosium was shown to be field dependent in the approximate temperature rarge of 90°K to l72'1c. Below about 90°K dysprosium appeared to be truly ferromagnetic, confirming the observa-tion of Trombe (21,22).
The magnitude of the measured values of the magnetic moment of
dy'~rosium indicates that the orbital angular momentum must contribute to the ferromagnetism.
An absolute saturation magnetic moment of at least 8 Bohr magnetons was indicated by the data obtained in the temperature range of 31.25°K
The strange behavior of the magnetization vs 1/H curves of dysprosium was noted, and possible explanations were set forth.
9. The magnetic moment of erbium was measured for applied fields of 43000-18~000 oersteds, and over the temperature range of 20.4°K to 7loK.
10. The Slsceptibility of erbium was shown to be field dependent below about 55°K.
11. Erbium appeared to be truly ferromagnetic at 20.4°K.
12. The magnitude of the measured values of the magnetic moment of erbium indicates that the orbital angular momentum must contribute to the ferromagnetism.
13. The similarities and differences of the m&gnetic behaviors of erbium and dysprosium were noted.
•• from the theoretical standpoint, these substances ~e rare earth rretals7 are much simpler than those of the iron group. Because the
4felectrons are deeply imbedded in the atom~ they do not wander
appreciably from the atom, and the question of band structure involved in Stoner's ncollective electron ferromagnetism" does not enter.
For this reason as much experimental info~ation as possible on the rare earth metals in highly desirable.
The recent development of processes at this laboratory for the sepa= ration of pure rare earth salts (1) and for the preparation of the pure metals (2) have made it possible to begin experimental researches on the magnetic properties of these elements here. This thesis is a report of the beginning of this experimental research.
The first significant advance in the theory of ferromagnetism2 was made by Weiss (5) in 1907. Langevin has by this time developed his well
known theory of paramagnetism, based on the assumpti'on that the orienta-tion of a molecular dipole of moment ,k( in a field H is governed by the
Boltzman distribution law. With this hypothesis it can be shown that the moment per unit volume is given by
M :: N~<AH/kT) D
where N is the number of molecules per unit volume, and L(x) is the Langevin function.
L(x) : coth x- x=
1Remark by J. H. Van Vleck at Colloque International de Ferromagnetisime et d~Antiferromagnetisime de Grenoble. See (21).
The basic assumption made by Weiss was that the effective field acting on the elementary magnet in a ferromagnetic substance was not the applied field H, but rather H + qM, where q is a proportionality constant, independent of temperature and called the Weiss molecular field constant. Substitution of H + qH, in place of H in the Langevin function in equation l)j yielqs
mere -pis the ratio of the magnetization to the absolute saturation magnetization, ~ o
This equation provides a theoretical justification for the experimen~ tal Curie-Weiss Law above the Curie point, and provided a semi-quantitative explanation for ferromagnetic phenomena below the Curie pointo
1)3 bye, using quantum roo chan,icaJ.. oo nsi derations, replaced the contin· -uous distribution in the Langevin theory by a discrete series of orienta-tions3 and developed the well knqwn Langevin-Debye theory of paramagnetism. When a similar extension is made to the Weiss theory, equation 2) becomes
...- _ B 2~(H + ql1)
where B5(y) is the Brillouin function
(?$1 ...Y.\ l
B5(y) : 25 coth 2S )- 25 '\25}
Here 5 is the spin quantum number of the atom and~ is the Bohr eh
The Debye-Weiss theory was somewhat successful in explaining the
reduced m~gnetization curves of iron, nickel, and cobalt, when the
para-meter 5 was chosen as one-half. The discrepancies between the theory and experiment have long been recognized, particularly in the neighborhood
of the Curie point.
In order to bring the theoretical and experimental reduced magnetiza-tion curves of iron, nickel, and cnbalt into better agreement, and to
explain the magnitude of the absolute saturation magnetization of these elements, Stoner's ( 6, 7) "collective electron theory of ferromagnetism",
Hhich is based on the band picture, was developed. However, as observed
by Van Vleck, th~s theory is probably not applicable to the rare earth
Bloch (8) has calculated the variation of the saturation magnetiza~
tion with temperature using a "spin=wave" treatment. For the low tempera
-ture approximation (Le.ll assuming that only the lowest energy levels
excited)~ he has shown that the saturation magnetization is linear in TJI2o
This has been experimentally verified for iron and nickel below 700K (9)o Above 70°Ks the experimental values of the saturation m:ignetization of iron9 nickel, and cobalt seem to have a linear T2 temperature dependence.
The large 11mole cular field" postulated by Weiss has been explained
by Heisenberg (10) as arising from the quantum zoochanical forces of exchange acting between electrons of adjacent atoms. It was necessary for Heisenberg to assume that this exchange energy be positive in order to favor the ferromagnetic state. In the high ternperd.ture range (Le • .9
above the Curie point)~ this theo:ry was also able to provide a theoretical understanding of the empirical Curie-Weiss Law.
The result of the Heisenberg calculation (assuming quenching of the
orbital angular momentum) ~as similar to equation 3) withy replaced by
and the Curie point was given by
Tc = 2JzS(S ~ ~
Here, z is the number of nearest neighbors~ and J is the exchange integral.
Recently (11) Zener has taken issue with the Heisenberg mechanism of ferromagnetism. He believes that the exchange interaction between the Jd electrons of neighbori.ng atoms in the iron group (presumably the 4f elec= trons in the rare earths) is such as to oppose ferromagnetism. He proposes that the ferromagnetic state exists only when the positive exchange inter-action between the valence electrons of neighboring atoms» which are
assumed to be strongly coupled so the 3d electrons, is larger than the
Slater (12.} also has recently attacked the usual approximation methods
of calculating ferromagnetic phenomenao He.has pointed out that these
methods, as they are USQally applied, are not appropriate for frystems
containing more than a few electrons. Slater maintains9
ooo that to treat magnetic problems properly3 we must make
such calculations (i.e.3 linear combinations of different
the energy of the states of different magnetizations as a func-tion of internuclear distance, and see which states lie lower~
the magnetic or nonmagnetico
Besides the usual paramagnetic, diamagnetic, and ferromagnetic
sub-stances~ there is still another class of magnetic materials, those which are antiferromagnetic. These substances Show experimentally a
monoton-ically increasing susceptibility >d th decreasing temperature.~ which reaches
a maximum at a cert~in temperature called the Curie temperature.l Below
the Curie temperature, the susceptibility decreases •nth decreasing tem-perature until at absolute zero the susceptibility is
0.85times its value at the Curie temperature. These substances also show dependence of the susceptibility on field strength, and hysteresis effects below the Curie temperature. The direct experimental test for antiferromagnetism is qy neutron diffraction studies.
The behavior of antiferromagnetic substances is explained
theoretic-ally in the i'o1Jowing way. The crystal is thought to be made up of two or more sublattices A, B, etc., such that the nearest neighbors of atom A
are atoms belonging to B and vice versa. In the Heisenberg molecular field, all the spins of neigh"50ring atoms are, on the average.:~ assumed to be parallel. This assumption would be valid if the exchange integral
1vere positive, as then the state with aligned neighboring spins would be the state of lowest energy. However, if the exchange integral is negative,
the state of lo;Jest energy i.s that in which the spins of lattice A are
c..ntipar&llel i;.o the spins of lattice B. If this
tvr:r:eof model is treated
by the metnod analogous to that used £or the Heisenberg model and
expres-sion i: obtained for the Curie temperature, and the Curie-Weiss Law for
the paramagnetic behavior above the Curie temperature is again obtained.
The decreasing susceptibility with temperature, and the field dependence of susceptibility below the Curie temperature is also understood on the
basis of this model. For more detailed descriptions of antiferromagnetism
and'the mathematical an~lysis, the reader is referred to the original
papers of Neel (13, 14), Bitter (15), and Van Vleck (16).
Unfortunately it has been impossible to calculate the sign of the
exchange integral for those substances of interest in magnetic phenomena. HN,rever~ Slater (17) has developed a qualitative rule for predicting the
possibil~ty of the existence of the ferromagnetic state for a given sub=
.stance. I t states that the necessary condition for the existence of
ferromaGnetism is that the atomic radius be small compared to the distance
bett·Jeen atoms. Presumably 3 therefore, when the ratio of R/r (the atomic
~~.,t"'?_~!:atio~~ver the radius of the unfilled shell which provides the bulk
lThe term "Curie temperature" will be used to designate the temperature
belmv- 1-rhich a m bstance is antiferromagnetic, as distinguished from the
of the magnetic moment) is small, the exchange integral is mgative9 and the antiferromagnetic state is favored. As the distance between atoms becomes larger (assuming that r remains constant), the exchange integral becomes positive at a centain critical distance of atomic separation. As
Ris further increased, the exchange integral also increases in the posi•
tlvedirection until a maximum is reached.
Afurther increase in
decreases the magnitude of the exchange integraL In this region of positive exchange9 the ferromagnetic and paramagnetic states are favored.
Briefly this is the present state of magnetic theor.y. In general, the theories of paramagnetism and diamagnetism (which were not discussed here) have been reasonably successful in both a qualitative and quantita-tive way. The theories of Weiss, Heisenberg, Stoner9 Neel, etc., have yielded a qualitative explanation of ferromagnetism and antiferromagnetism. Perhaps it is due only to the difficulty of the calculations involved in these theories that they are not also completely satisfying from a quan-titative standpoint. Nevertheless, qy supplying new and more complete data on the ferromagnetic rare earths,~~ there is hope that a more complete understanding of magnetic phenomena will be obtained.
Three rare e drth metals were chosen for this study: gadolinium, dysprosium, and erbium. These metals were selected because they were either known to be ferromagnetic, or tll ere was good reason to believe they were ferromagnetic.
The ferromagnetic properties of metallic gadolinium were reported in 1935 by Urbain, Weiss and Trombe (18), and by Trombe (19). The value of the absolute saturation magnetization was cited as
353.5cgs units, and the Curie point as 16°C.
Preliminary measurements on gadolinium were made using a ballistic method with the sample in the form of a torus (20). Since there appeared to be certain discrepancies between these preliminary measurements and those reported by Trombe, it was deemed desirable to extend these
measure-:rre nt s to higher fields.
Dysprosium has been shown by Trombe (21, 22) to be ferromagmtic. He reported the existence of a magnetic anomaly at 179°K. From 179°K to l05oK he noted that the susceptibility was field depend~nt. Below 10~°K, dysprosium was truly ferromagnetic,~~ having a Curie point at about 105 Kp Trombe did not &Lve in his papers a value for the absolute saturation magnetizationi or magnetic moment vs. magnetic dysprosium were l_llade.
Neel (23), working with the magnetic susceptibility data of Klemm and Bommer (24), predicted a Curie point for erbium at about 40°K. Barsonis (20) work on the electrical resistivity of erbiun has shown an anomaly at a bout 70°=·80°K. This type of anomaly in the electrical resis=
that hope of finding a new ferromagnetic element, erbium was chosen as the final substance to complete this initial investigation of the magnetic properties of the'rare earth metalso
Of all the measurable quantities of a ferromagnetic substance9 only the saturation magnetization, and in particular only the saturation magnetizationat absolute zero is alone characteristic of the substance. All other magnetic quantities such as the Curie point, coercive force9
remanent magnetization, etc., are dependent to a greater or lesser extent on the past history of the substance. Consequently the primary purpose of this investigation was to determine, if possible, the absolute
saturati. on magnetization of the three elerrents chosen.
For comparison of experimental data with theory, the variation of spontaneous magnetization, i.e., the magnetic moment of a substance in a zero applied magnetic field, is required. The spontaneous magnetization can be determined fromthe data obtained in this investigation, but empha~ sis has not been placed in this direction.
The value of the Curie point is also required to correlate experimental data with theory. In the past i t has been the custom to define the· curie point in two different ways. Probably the preferred definition is the temperature at which ~pontaneous magnetization disappears. The second definition is the temperature at which ferromagnetism disappears in a small, but not vanishing, applied field. Which definition is used seems to depend upon the experimenter and his rrethod of measurement.l In the measurements of the Curie point of gadolinium reported here, it would appear that these two definitions are not synonymous.
IIIo EXPERIMENTAL PROCEDURE
The rootals used in this investigation were ru bjected to spectro~ graphic analysis to determine the amount of impuri ties2 in parts per million of the following elements: iron, nickel, cobalt, calcium, and other rare earths.
The analysis of the gadolinium metal used was as followB: ca, detect':l-ble but le.ss than 200 ppm; Sn, detectable but less than 600 ppm;
1Trombe (18, 19) uses the latter definition for the Curie point determina-tion of gadolinium. He does not state how the Curie point was determined for dysprosium
(21, 22).For an example of a Curie point determination using the former defin~tion, see
Co3 Ni~ and other rare earths9 not detectedo
Dysprosium ::h owed the following impurities: ca:J detectable but less then 100 ppm; Fe~ detectable but less than 2000 ppm; .Mo, detectable but less than 2000 ppm; Er, detectable but less than 200 ppm; Y3 detectable
but less than 200 ppm; Ni, Co~ and other rare earths not detected.
The erbium analysis showed~ Ca9 detectable but less than 100 ppm;
Y, detectable but less than 100 ppm; Fe~ detectable but less than 2000 ppm; Ni~ Co~ and other rare earths not detectedo
Crystal structure studies of gadolinium.9 dysprosiuq, and erbium were
made at this laboratory concurrently with the magnetic studies (26). The
results of this investigation showed the three metals to be hexagonal
close packedo The temperat.ure ranges over which the structures were
investbgated were~ gadolinium l30-345°Ky dysprosium 47-300°K, and erbium 41-300 K.
Bo Method of Measurement
Magnetic moments in this investigation were determined by plcicing the sample in an inhomogeneous magnetic field and measuring the force exerted on the sample in the direction of increasing field strength. It can be shown (27) that the rnugnitude of this force is given by~
where F ~ the force in the X=·direction, m ._:, the mass of the sample9
cr ~ the magnetic moment per unit mass, and
dH/dx :;:: the magnitude of the gradient of the md.gnetic field in the x=directiono
For the purpose of discussion3 the direction of the rra.gnetic field will be designated as the horizontal or y~directiono The gradient of the field and the force are at right angles to the field and are in the
vertical or x=direction.
The magnet used in this study was a 20 kw Weiss-type electromagnet,
capable of producing a 202000 oersted field in a 1! inch pole gapo
The gradient of the field of the electromagnet was calibrated using a sample of 99o99 per cent pure iron9 supplied by Johnson~ Mathey and
applied fields greater than 4000 oersteds. 1 The saturation magnetization
at 20oc for this somple was taken to be 217.8 cgs units (28). The cali~
bration was cheeked using a sample of nickel
99.97per cent pure and
assuming a saturation value of 54.65 cgs units (28). The two separate
calibrations agreed to at least 0.8 per cent over the entire range of
The inhomogeneous field was produced by a method suggested by
(29).The vertical faces of ordinary 60° truncated conical
pole pieces were divided into three horizontal sections of equal width
(see Figure 1). The upper and lower sections were connected by the middle
section ..rhich ~·.ras machined at about 5° from the verticaL A portion of
the field uas found v1here the gradient uas almost constant over nearly a
half~inch; thus.~ the sample uas in a position of stable equilibrium during
the lveighing process. The magnitude of the gradient produced by this technique varied from 100 oersteds per em. at low fields~ to 1000 oersteds
per em. at high fields.
The use of the Sucksmith-type pole pieces offered three advantages over an inhomogenous field produced by the fringing field of ordinar,y
60° truncated conical pole pieces. First~ it allowed the full use of the
maximum field strength of the magnet~ as the sample was placed in the
middle of the pole gap (position A, Figure 1) rather than at the edge of
the pole gap (position B~ Figure 1) where the magnitude of the field has decreased considerably.
The second advantage was that the Sucksmith pole pieces provided a larger area over vmich the gradient of the field was nearly constant. This larger area of constant gradient allowed for faster and more accurate measurements.
The third advantage was that it virtually eliminated the x-component
of the force caused by image poles (30). This force is proportional to the permeability of the iron in the magnet and to the square of the total magnetic moment of the sample. In Figure 1 the approximate position for
the image pole is designated for the tvm positions, assuming that the iron
~~-~~~gnet _hcl. s
a.z:_infinite permeability. The use of the Sucksmi. th~·type
lin various sections of this dissertation~ values of magnetic moments are cited which were obtained in applied fields of less than 4000 oersteds. No claim is made for the accuracy of the aboolute magnitude of these values. It is to be noted~ however, that since iron is far all practical purposes saturated (to within 1 per cent) for applied fields greater than 1000 oersteds, the error in the magnet calibration in this range is not
2This difference between the t>vo calibrations using different standards
is within the standard deviation of the repeatability of a number of
N S c==:::J
- - c::::=::J
Figure 1. The Sucksmith-type pole pieces used in this stuqy. sample position A is position used. Position B
is sample position used if ordinary truncated conical
pole pieces are employed. Points 5' are approxi.m:1te
pooitions of image poles for sample positions A and B,
pole pieces thus reduces any x-componeht of the image pole force that may
be present by approximately a factor of 10 (i.e., sin 5°/sin 6o0~.1).
The proportionality factor of the image pole due to the perrneabili ty
of the m'lgnet is automatically taken into account in the magnet calibra
-tion3 and does not introduce false measurements in either technique. The proportionality factor due to the total magnetic moment of the sample can not be so easily dismissed. The best one can hope for is that the x=com
-ponent can be reduced to the point that it can not be detected by the force measuring device used. The Sucksmith-type pole pieces essentially
do this. The fact that it was possible to obtain the saturation magnetiza~
tion of nickel to within 0.8 per cent of the accepted value when the magnetic field was calibrated with iron, mowed that the x-component of the image pole force was independent (i.e., not detectable by the measuring apparatus) of the magnitude of the total magnetic moment 'When the moment was varied by a factor of four.l Since the magnetic moments measured to determine the absolute saturation magnetization in this investigation are
comparable to that of iron (within 15 per cent), the image pole force did
not limit the accuracy of these measurements.
The magnetic field was measured using a Rawson rotating coil flux-meter.
The calibration samples and the rare earth metal samples were in the form of cylinders, 10 mm long dnd 1 mm in diameter. The magnetizing field
was calculated using the expression
H : H0 - NI,
the magnetizing field,
the applied field,
the magnetization per cm3, and
the demagnetizing constant, taken to be
0.0875 for samples of the above aspect ratio (31).
Two methods were used for the Curie point determination of
gadolin-ium. In the preliminary measurement, with the torus, the variation of the nagnetic moment with temperature was observed for a sn.all constant
field. The second method was to observe the variation of the spontaneous
magnetization with temperature, using fields produced by the electromagnet. The spontaneous magnetization was determined by the extrapolation
tech-nique of Weiss and Forrer (28).
The Curie points of dysprosium and erbium were determined in a nanni~r to be discussed later.
lrn various sections of this dissertation, values of magnetic moments are
The cryogenic apparatus consisted of a double metal dewar (Figure 2).
The sample was placed in the inner dewar, ::l.nd the temperature of the sample
was controlled by a stream of helium gas. The outer dewar contained a
heat exchanger and a liql id bath. Helium gas W.iS cooled in the exchanger,
then mixed with a stream of warm helium before enteringthe inner dewar.
The temperature range from 26-85~ was obtained with a hydrogen bath, from
85-230~ with nitrogen, 200=280°K with acetone and d~ ice9 280-310°K with
ice water. The temperature was controlled to within a degree for satura
-tion measurements and to within a quarter of a degree for the Curie point determinationJ using spontaneous magnetization data.
The temperature was measured by a copper-constantan thermocouple cali
-brated against a Bureau of Standards calibrated platinum resistance
This apparatus was used throughoutj except for the 20.4°K data.
Here tre sample was imnersed directly in the liquid hydrogen bath9 and
the necessa~ buoyancy corrections made to account for changes in the height of the liquid.
The Curie point determination m-.1de "1-ti. th the torus was performed in·
an alcohol bath and the temperature was controlled to within O.OS°C. A
mercu~ thermometer which gave readings of the true temperature to
.o. 0.1oc was used to rreasure the temperature.
Figure 3 shows several of the representative curves of the isothermal
variation of the magnetic moment as a function of 1/H for gadolinium. It
was found that the variationj far magnetizing fields of 4,000-189000
oersteds over the temperature range of 20-253°K, was well represented by the expre ssi. on
where C"'H9 T :::: the magnetic morrent per gram_,
o-<l"J T :: the saturation moment per gram at T°K9
H :;:: the magnetizing f i eldj and
a - constant.
Figure 2. Cryogenic apparatus used to provide temperature
10 300 90 80
20 10 300 90 80 70
1- 2!10 ~---·----,---"---.---o-;;~!!6'•!S:-K-<>----o---o----_j200
.;%· !57ft ~
~ 20 --- 13~ 20
~I 0 1=--- 1!!0.!¥1< I 0
- 90 ---~~--~---~~m~~~---~
~ 80~---v----~----~l:!~OT~'·~OL~~---~ 80
2 70 70
60---~--~----~--~~2~3~1.4~~~~--~---~ 60 I !10 40 30 20 10 100 90 10 20
70 0 0.1 0.2 0.3 0.4 0.!1 0.6 0.7 0.8 0.9 1.0 1.1 1.2 1.3 l4 1.& 1.6 1.7 1.1 1.9 70
"HI 104 OERSTEDS1
The data were extrapol~ted to 1/H equal to zero, using the method of least squares to find the saturation magnetization.
The val\lB of the saturation magnetization obtained by the above extrapolation, are plotted as a function of TJ/2 in Figure 4a. It may be observed that the data seem to agree quite well over the temperature range examined with an expression of the form
crC>D 3 T :
o-oo3 o(l - bT3/ 2)
rroa!l 0 ~ the absolute saturation magnetization.:~ b - a constant, and
T ~ absolute temperature.
It may be further observed (Figure 4b) that the data agree fairly well with the expression
=cr -oe> o(l - b~)
' ' 0
between 2.50°K and 130°K.? but the data
~eemto fit the
~/2 expression at lea.st as well if 3~t better than the T expression over this range.
Con-sequently.? the T law w~s used over the entire range for determining the absolute saturation magnetic moment.
Using again the method of least squares3 the value of the saturation magnetization at absolute zero was found to be 2.53.6
f0.9 cgs units. This saturation moment corresponds to 7.12 Bohr magnetons where the value
used for the Bohr magneton was .5.587 emu per mole (31).
In Figure .5 the ratio of a-~ T/o-:~ is plotted as a function of the
ratio of T/9, where
eis the Curie temperature. Several curves.? obtained
from the :Debye-Weiss theory of ferromagnetism for various J values9 are also mo:wn. To make comparison between experi~rental data and the
Debye-Weiss theorY.~ the ratio of a-0 , T/C!O, o, where
o-09 T is the spontaneous
magnetization3 should be plotted as a function of T/9. However3 the value of the spontaneous magnetization differs from the saturation m:l.gnetiza-tion for gadolinium by only a few per cent3 which would not change the
location of the plotted points significantly.
The variation of the square of the spontaneous magnetization with temperature near the Curie point is shown in Figure 6b. The intersection of the extension of the nearly linear portion of' this curve with the temperature axis was taken to be the Curie point, i.e • .? 17.7 ~ O.J°C.
4(a) The saturation j<3-2netic moment of gadolinium as
0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0
5.The reduced magnetization curve for
gadolinium; also, the th~retical curves
=7/2 and J-oa, from the Debye-Weiss quantum theory of
-0 8~~9~~~.-1~12~1=3~14~1=5~~~~·~1=9-2~0--2-1~22. 0
Figure 7 shows a number of the isotherrt\S of the magnetic moment of
qysprosiurn as a function of applied field. Figure 8 is an enlarged portion of the low field region of Figure 7. The initial susceptibility (i.e., the susceptibility calculated from the low field9 linear portion of the curves in Figure 7) from ll3°-202°K plotted as a function of
temperature is shown in Figure
9.One notes that for applied fields up to 189000 oersteds the
ovs. H isotherms remain linear down to about 17S°K. Below 17S°K, the isotherms are linear in the low field region3
but at some higher field the susceptibility becomes field dependent.
As the temperature is lowered below 17S°K, the field for which the suscepti-bility becomes field dependent i& smaller.
Below ll0°K the magnetization curves for dysprosium are much the
same as those for gadolinium, and are typical of a ferromagnetic substance.
It is observed that the element is very magnetically 11hard11 in comparioon to iron or even gadolinium, and is far from saturation in a field of 18,000 oersteds. One also notes that below 103°K, dysprosiwn becomes rapidly temperature saturated, i.e.9 temperature has little effect upon the magnitude of the rnagnetizationo
The 20.4~ data deserve special notice. The curve falls far below the 31.2SOK isotherm. These data were taken by a different method from the other isotherms as pointed out above. It has not been possible to overlap the temperature ranges of the two rrethods, hence it is not possible to state unequivocally that the anom:lly is real; one might attri1:ute the result to fault in one of the methods of rreasurement. I t is to be
noted, however, that no such inconsistency was evident in the data for gadolinium at 20.4°K.
The anomaly observed by Trombe is quite evident in Figure 7 and in Figures 8 and 9. The general shape of the curve in Figure 9 above 1SS°K
is not unlike the corresponding curve for an antiferromagnetic substance
in the neighborhood of its Curie temperature.
In order to discuss the magnetic behavior of dysprosium9 three or
possibly four temperature regions or magnetic states may be distinguished. The first state, P, occurs above 176°K vlhere the element appears to be
truly paramagnetic. The second state (hereafter called state A1) occurs
in the temperature range bounded
qythe anomaly at 1760K and
ferro-magnetic Curie point at about 92°K. (The Curie point determination i s
discussed below.) The magnetic behavior of dysprosium in this tanperature range is characterized b,y the field dependence of the susceptibility, and
2 5 4 5 I 7 I 9 10 II 12 15 14 15 II 17 II It 20
H X 10·1 OERSTEDS
172D-K - - - - 4
/h168...-K - - - - 5
~/,/¥"153.4•K - - - 6
13~K - - - - 7
121.0-K - - - - 8
113.0•K - - - 9
8.An enlarged plot of the low field region of Figure
showing the anomaly in dysprosium observed by Trombe.
.6 ..~---, ~
> ~ 5 .
The third magnetic state of dysprosium (hereafter called state F), occurs belorr aoout 92°K. Here the element appears to be in a true ferro-magnetic state, characterized
qyspontaneous magnetization, saturation effects, and by hysteresis effects.
A fourth magnetic state may exist for dysprosium (hereafter called state A2) in the temperature range below about 25°K as indicated by the anomalous behavior of the 20.4°K isotherm.
The difficulty encountered in attempting to obtain the Curie point of state F from spontaneous magnetization data may also be seen from the magnetization curves (Figure 7). In order to determine the Curie point by this method, it is necessary to obtain spontaneous magnetization data as a function of temperature from the !1'k3.gnetization curves above and below the Curie point. Because of the strange behavior of dysprosium immediately above its Curie point (i.e., in state A ), it was found impossible to
obtain spontaneous magnetization data
~ichwere complete enough to allow an accurate determination of the Curie point by this method.
In Figure 10 the CUrie point is determined by extrapolati. on of the linear portion of theOJ.200 vs. T curve to the tanpe~ature axis. The
o-1200 data were obtaine
a.in a relatively weak field of 12 00 oersteds. The value of the Curie point determined by this method is 92°K. Because the Curie point is somewhat dependent on the value of the applied field used in its determination, 92°K is probably several degrees higher than the value of the CUrie point determined in a nearly zero applied field.
Figures 11, 12, 13 and
14are plots of the magnetic moment vs 1/H for several of the isotherms of Figure 7. These curves differ consider-ably from the corresponding curves of gadolinium. The curves in the neighborhood of l00°K are nearly linear above 5,000 oersteds. At temperatures above l00°K, the curves are concave downward. The curves below 80°K seem to consist of two nearly straight intersecting lines.
Both of the linear section$ of these curves have been extrapolated to infinite fields to obtain the saturation moments. No attempt was made to use the method of least squares in these extrapolations.
rn Figure 15 the saturation momenti obtained from Figures 12, 13, and 14 are plotted as a function of T3
Z(the 20.4°K data have not been considered) to obtain the absolute saturation moment. The saturation moment at absolute zero for dysprosium appears to be about 299 i
5cgs units if one uses saturation moments from the high field extrapolations, and about 273 ~
3cgs units, if one uses the low field extrapolated saturation moments. These moments correspond to
~ \ \
Figure 10. The Curie point determination for dysprosium state F
103.0-e< 113.o•K 121.0°K
~ 100 168.o•K
C) C( 2
.I .2 .3 .4 .5 .6 .7 .8 .9 12 1.3 1.4 1/H X 1040ERSTEDS-1
360 50 40 30 20 ....
~ C) ~ w n. ...__ ... ...
...z w ~ 2:
---... ..._ ..._ ----~
z C) 20 4 ~ 0 200 90 lBO 170
0 .I 2 .3 l4 5
.8 .9_, OERSTEDS
Representative curve of the isothermal variation of the
magnetic moment of dysprosium as a function of 1/H.
T= 31.25° K
1.0 1.1 1.2 1.3 14 1.5
Figure 13. Representative curves of the isothermal variation of the magnetic moment of dysprosium as a function of 1/H .
-T = 35° K
UJ29 v v
20 10 2000
.I .2 .3 4
T:: 50° K
.5 .6 .7 .8 .9 1.0 1.1 1.2 1.3 1.4 1.5 1.6
1fX 104 OERSTEDS-1
Figure 14. Representative curves of the isothermal variation of the
-magnetic moment of dysprosium as a function of 1/H.
-i:;x 104 OERSTEOS- 1
(!) 6 c:t
-- -- --X X
It is to be noted that these absolute saturation moments were obtained
using data from the temperature range of 3l0-80°K only, and therefore only
attempt to point out what the approximate ~gnitude of the saturation
moment at dbsolute zero •wuld be assuming that no further anomalies occur
between 0°·~31 °Ka
Figure 16 sho1..rs several of the ffi:ignetic isotherms for erbium. Above
about 55°K erbium is paramdgnetic as indicated
qythe linear magnetic
isotherms at 7l.0°K and 61.2oK. Below 51°K (state ~) its susceptibility
becomes field dependent~ but there is no evidence of spontaneous
ffi:ignetiza-tion. At the hydrogen point erbium seems to be in a true ferromagnetic
sta.te (state F)o The extreme magnetic "hardness11 of this state is to be noted.
The similarity of the magnetic behavior of ·erbium and dysprosium is
quite evident. Howevers the anomaly associated \vi th state A1 of dysprosium
is not apparent in the corresponding state of erbium (see Figure 16~ where
the initial susceptibility of ertium is plotted as a function of tempera
-ture). It may be that the measuring apparatus was not sensitive enough
to allm·T the obser,rati on of the anomaly7 or that the wrong temperatures · . ..rere chosen; but, in any case~ i t is apparent that the anomaly is not as
"1-lell developed in erbium as in dysprosium~ if it exists at all.
The temperature at which the su.sceptibility of erbium becomes field
dependent may be cited as 56.,0 ;:, 5°K"
The a- vs., l/H rurve :·or the 20.4c'K data ol' erbium is quite similar
to those of dysprosium.. Tha.t is, the curve seems to consist of two
intersecting straight lj nes. Extrapolation ol' the high field region of
this curve to 1/H :-:: 0 indicates that the saturation magnetization of
erbium at 20.4°K is· of the Ol'der of 286 cgs units, corresponding to
about 8.6 Bohr magnetons per o:J.tom"
Eecause of the incompleteness of the data.~~ no attempt has been rrade
to determine experimentally the ferromagnetic Curie point of state F~ nor
was it posclble to determine the absolute saturation moment of erbiumo
Ass~ming a lii,aw of Corresponding Status" to be valid for erhlum and
dysprosium~ the ferromagnetic Curie point of erbium mdy be estima.ted.
Usine the temper.::J.t'.lre d.t "1-Jhich the susceptibilities of dysprosium and
erbium become field de~endent (i.e" 9 176°K and 56°K respectively)~
0 c 2
•7 I I 10 II lit I:S 14 15 II 17 II II ItO
H X 10-:s OERSTEDS
Figure 16. The magnetic monent of erbium as a function of applied
Figure 17. The initial susceptibility of erbium in ihe temperature range
V. DISCUSSION OF RESULTS
Of particular interest is·the fact that the value of the absolute saturation magnetization obtained by Trombe by extrapolation of a T2 plot
a~rees exce3_%ngly well ••~th the value ?btained here using an
extra~ola-tlon of a T plot. Of lnterest also lS t~e fact that the saturatlon
orgddolinium is linear in T3/2 over nearly its entire
ferromagnetic range. Gadolinium thus seems to be peculi_,_r in t.h.is respect
as ferromagnetics, other than the rare earths, are linear in T3/2 only
at very low temper~ture~.
This investigation also showed that gadolinium is not as magnetically "hard" as indicated by Trombe, although considerably "harder" than iron. The constant (a) in equation 6) is an indication of this "hardness" and
has the value of about 170 oersteds from the data reported here. This
is to be compared with Trombe1s value of 1350 oersteds (for iron, a~lO
oersteds). This difference of "hardness" between samples studied here
and Trombe' s was also indicated by the preliminary measurements at low
fields (20), using the ballistic method.
The Curie point found by the ballistic method, Figure 6a~ agrees
quite well with Trombe's value, where he has defined the Curie point as
the temperature at "1-lhich ferromagnetism disappears in a small field. The
Curie point is found to be some t•vo degrees higher when it is defined as the temperature at which spontaneous magnetization disappears. The
disagreement bet••een the values of the Curie points does not seem
unreason-able when the differences in their definitions are considered.
It was possible to repeat the data obtained by the ballistic method
irrespective of whether the Curie point vlas apprQC.tched from above or
below, showing there was no temperature hysteresis (within at l~ast 0.1 °)
at the Curie point.
It should also be mentioned that there was found to be no shift in
the Curie point due to annealing. Such a shift was indicated by Curie
point determincJ.tion by electrical resistivity measurements on gadolinium
at this laboratory (32). However, there is no definite assurance that the samples used for magnetic measurements were not previously annealed
in the casting process.
It ~y be observed that the absolute saturation magnetization is some
2 per cent higher than vmuld be predicted i f only the spins of the
electrons contributed to the magnetization; this deviation is believed to be outside the experimental error. Also.)) the reducgd magnetization data
state using the Debye=Weiss theory of ferromagnetismo Had o 0 T data been used for this plot rather than a-~'T' data~ the experimental points would have been slightly lower than the points showno
The experimental results of the magnetic properties of dysprosium
are probably the most interesting of the three elements studied. Although
the magnetic behavior is very complicated3 and is far from being
under-stood theoreticd.lly, it is felt that the above experimental data will
eventually have a significant effect on the theory of ferromagnetism.
The high magnetic moment of dysprosium is of considerable theoretical significanceo Magnetic moments have been measured of the orQ.er of 245 cgs units for dysprosium. Such a magnetic moment corresponds to about
7 Bohr magnetonso The spectroscopic state of the dysprosium ion is a
2J and.~ from the paramagnetic theory of Hund and Van Vleck (4) ~
(w.1ere it is assumed that the ions are essentially free), one would expect an acsolute saturation magnetic moment of 10 Bohr magnetons. These data indicate that the absolute saturation moment of dysprosium is probably
not this large. This may be interpret,ed as meaning that, the
are not completely free from the influence of neighboring atoms.
On the other hand.., it has been necessary to assume in the case of ironj nickel, and cobalt9 that the orbi ta.l angular monentum was almost
completely quenched, in order to explain the magnitude of their absolute saturation l'l'ldgnetization. If the orbital moment were completely quenched
in dysprosium~ one would expect a saturation moment of 5 Bohr rnagrntons.
The absolute saturation moment is obviously much larger than this~ as measured values of the magnetic moment larger than 5 Bohr l'l'ldgnetons have been found in regions ·...rhere the element is far from saturation. This is the first pure metals to the au thorns knowledge, in wh l ch orbital angular momentum has been mown to play a definite part in ferromagnetic proper~ ties.
Quenching of the orbital angular momentum is2 of course~ due to the
proximity of neighboring atoms im the crystal lattice. Since i t appears that the quenching is far from complete in dysprosiumj one is forced to assume that the atoms are nearly free.9 at least as far as the
are concerned. The effect of this conclusion on the magnitude o.f the Heisenberg exchange integral is not obvious.
The unusual shape oJ' the magnetization vs 1/H curves must be
explained. Perhaps a possible explanation can be made in ter~ns of a sys-tem of t 1'110 magnetic phases. The general sha.pe of the curves could be
A crystal structure change could be a possible mechanism for a system of two magnetic phases. Because of the X-ray investigation of dysprosium over the ferromagnetic range
(26),this mechanism seems unlikely.
An impurity such as iron surrounded by dysprosi. um might be another
mechanism for the ~stem. The spectrographic analysis for iron showed less than 2000 ppm, but, as no quantitative standards for iron were yet available, this was given as a maximum limit for the iron impurity.
The iron cerium intermetallic compound has been found to have a
serious effect on the magnetic properties of cerium metal. Several of
these compounds are known to be ferromagnetic and in particular compounds
with as low as 100 ppm concentration of iron are believed to be
ferro-magnetic, having a Curie point somewhere bet1-1een
Whether the iron impurities are serious in dysprosium and erbium,
and whether iron is the cause of the apparent system of two magnetic
phases, will be answered only after better quantitative methods of analysis
have been developed and controlled experiments performed.
One further mechanism for a system of two magnetic phases is the
possibility that dysprosium is ferromagnetic in one temperature range and
antiferromagnetic in another.
Before attempting to explain the magnetic phenomena of dysprosium
and ~rbium on the basis of such a system it would perhaps be wise to
recall several important facts about magnetic systems. First, if the
system is in its lowest energy state when the spins of neighboring atoms
are parallel, the substance is ferromagnetic. If the system is in its
lowest energy state when the spins are antiparallel, the subqtance is
antiferromagnetic~ Which of these energy states is lowest depends on
the coupling constants involved with nearest neighbor and next nearest
neighbor ~toms. Thus, there is no ~ priori reason why a ferromagnetic
ssstem can not be changed into an antiferromagnetic system just by
chang-ing the distance between neighboring atoms. Also there is no ~priori
reason why the difference in energy between the antiferromagnetic system and ferromagnetic system can not be small. Second, it is an experimental fact that some lattice parameters of some ferromagnetic substances
increase as the temperature is decreased through the Curie point. This
increase continues with decreasing temperature until the substance reaches
nearly its full saturation magnetization. At this point the coefficient of thermal contraction once more becomes dominant, and as the temperature is further decreased, the lattice parameters once more decrease. Similar changes in some of the lattice parameters near the Curie temperature have also been observed for antiferro~agnetic substances
1See Banister's work on gadolinium
(26)or the discussion in Bozorth
Banister. (26) has suggest,ed a possible explanation of the increase
of the 1a ttice pararreters (Le • .:~ the c axis for the rare earths) near
the Curie point. He notes that the in~eracti on between the 11mole cular
field" (assumed to be in the c0 direction) and 5d electrons would tend to
increase the probability of the 5d electrons being in a plane perpendicu=
lar to the c0 axis. The strength of the bond between neighboring atoms
in the c0 direction would then be decreased as the density of the electrons
(which essentially determines the strength of the bond) between these
two atoms would be decreasedo Since the strength of the interaction
depends upon the magnitude o.f the "molecular field119 which in turn depends
upon the magnitude of the rr~gnetizationJ the effectiveness of the bond will continue to decrease until the 11moleculi r field" becones nearly
con-stant9 or in other wordsj until the substance has reached its saturation
magnetization. When the substance has reached its saturation magnetiza=
tion the coefficient of thermal contraction once more becomes dominant
and the parameter begins to decrease once moreo
With the abqve facts in mindj it is now possible to suggest another
mechanism for a system of two magnetic phases to explain the magnetic
behavior of qysprosium.
As can be seen from B:.mistera s X~ray data on dysprosium (Figure 18L
the c0 axis tends to decrease as the temperature is lowered from room
temperature until a minimum is reached in 4he neighborhood of l75°K. It
is now supposed that dysprosium is in an antiferromagnetic statej' d.S
indicated by the form of the magnetic anomaly9 and by the fact that the
susceptibility is field dependent only for high fields. The antiferro~
magnetic arrangement of atoms may be like that suggested by Yin-Yuang Li
(36). As the temperature is further decreased t~e c0 axis tends to
increase.? which is in the direction such as to favor ferromagnetism. If
now the energy separation between the antiferrom.agnetic state and ferro=·
magnetic state is snull9 then one would expect that, the crit.ical separa=
ti.on distance between atoms would soon be reached by the expanding c0
axis. At about 92°K this critical distance presumably has been reached.~~
the exchange integral changes sign9 and the lowest energy state of the
system is such that the ferromagnetic state i~ favored. As the tempera=
ture is lowered further the ratio of R/r becomes more and more favorable
to the ferromagnetic state as the c axis continues to increaseu Below
the ferromagnetic Curie point at 928K the ma.gnetic isotherms (Figure 7)
begin to fall closer and closer together indicating that qysprosium is
near~ saturated temperature~w.ise. In this temperature region the coeffi~
cient of thermal contraction once more becomes domi.nant as expected9 and
again the c0 axis begins to decrease in the direction favorable to the
antiferromagnetic stateo From Banisteras data one would expect ·that the
critical distance.~~ which determines the si.3n of the exchange integral9
would be reached in the neighborhood of 40 K. Act1,1ally the magnetic data
shows that the critical distance is rec1ched around 200K. Thus.)l the
apparent anomaly at the hydrogen point observed in dysprosium is an indi
T I H
Figure 18. Variation of the lattice parameters of dysprosium with temperature (after Banister).